High-temperature behavior and structural studies on Ca14Al10Zn6O35
Kahlenberg, Volker; Krüger, Hannes; Zeitschrift für Kristallographie 237 (2022) 219–232; doi:

data_3000336
_publ_section_title
;
 High-temperature behavior and structural studies on Ca14Al10Zn6O35
;
_journal_name_full               'Zeitschrift f\"ur Kristallographie'
_journal_page_first              219
_journal_page_last               232
_journal_volume                  237
_journal_year                    2022
_chemical_formula_sum            'Al10 Ca14 O35 Zn6'
_chemical_formula_weight         1783.14
_space_group_IT_number           196
_space_group_name_Hall           'F 2 2 3'
_space_group_name_H-M_alt        'F 2 3'
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      196
_symmetry_space_group_name_H-M   'F 2 3'
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4.5
_audit_creation_date             2021-12-05T18:25:13-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.9278(6)
_cell_length_b                   14.9278(6)
_cell_length_c                   14.9278(6)
_cell_measurement_reflns_used    8703
_cell_measurement_temperature    873(2)
_cell_measurement_theta_max      29.16
_cell_measurement_theta_min      2.36
_cell_volume                     3326.5(2)
_computing_cell_refinement
;
        X-Area Recipe 1.33.0.0 (STOE, 2015)
;
_computing_data_collection
;
        X-Area WinXpose 2.0.22.0 (STOE, 2016)
;
_computing_data_reduction
;
        X-Area Integrate 1.73.1.0 (STOE, 2018)
        X-Area LANA 1.73.2.0 (STOE, 2018)
;
_computing_publication_material
;
STOE & Cie GmbH, X-Area, software package for collecting single-crystal or
multi-domain crystal data on STOE area-detector diffractometers, for image
processing, for the correction and scaling of reflection intensities and
        for outlier rejection, version 1.84, Darmstadt 2018
;
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SIR2004 (Burla et al, 2005)'
_diffrn_ambient_temperature      873(2)
_diffrn_detector                 'image plate (34 cm diameter)'
_diffrn_detector_area_resol_mean 6.67
_diffrn_detector_type            'STOE Imaging Plate'
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device       '2-circle diffractometer'
_diffrn_measurement_device_type  'STOE IPDS II'
_diffrn_measurement_method       'rotation method, \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0234
_diffrn_reflns_av_unetI/netI     0.0088
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            6799
_diffrn_reflns_theta_full        29.16
_diffrn_reflns_theta_max         29.16
_diffrn_reflns_theta_min         2.36
_diffrn_source
'sealed X-ray tube, 12 x 0.4 mm long-fine focus'
_exptl_absorpt_coefficient_mu    6.812
_exptl_absorpt_correction_T_max  0.1666
_exptl_absorpt_correction_T_min  0.1026
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
STOE X-Red32, absorption correction by Gaussian integration, analogous to
P. Coppens, "The Evaluation of Absorption and Extinction in Single-Crystal
Structure Analysis", published in: F. R. Ahmed (Editor), "Crystallographic
        Computing", Munksgaard, Copenhagen (1970), 255 - 270.
Afterwards scaling of reflection intensities was performed within STOE LANA.
J. Koziskova, F. Hahn, J. Richter, J. Kozisek, "Comparison of different
absorption corrections on the model structure of tetrakis(\m~2~-acetato)-
diaqua-di-copper(II)", Acta Chimica Slovaca, vol. 9, no. 2, 2016, pp. 136 - 140.
Finally a spherical absorption correction was done within STOE LANA.
;
_exptl_crystal_density_diffrn    3.56
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       fragment
_exptl_crystal_F_000             3480
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.142
_exptl_crystal_size_min          0.1
_refine_diff_density_max         0.385
_refine_diff_density_min         -0.402
_refine_diff_density_rms         0.089
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.01(2)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.216
_refine_ls_hydrogen_treatment    .
_refine_ls_matrix_type           full
_refine_ls_number_parameters     55
_refine_ls_number_reflns         763
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.216
_refine_ls_R_factor_all          0.0209
_refine_ls_R_factor_gt           0.0194
_refine_ls_shift/su_max          0
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0281P)^2^+11.1389P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0512
_refine_ls_wR_factor_ref         0.0546
_reflns_number_gt                752
_reflns_number_total             763
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            Ca14Al10Zn6O35_600C.cif
_cod_data_source_block           shelx
_cod_depositor_comments
'Releasing structure 3000336 into public domain as published material.'
_cod_database_code               3000336